Characteristics Optimization of Different Welding Processes on Duplex Stainless Steels Using Statistical Approach and Taguchi Technique - A Review Guide
International Journal of Engineering Inventionse-ISSN: 2278-7461, p-ISBN: 2319-6491Volume 2, Issue 3 (February 2013) PP: 26-34www.ijeijournal.com P a g e | 26Characteristics Optimization of Different WeldingProcesses on Duplex Stainless Steels Using StatisticalApproach and Taguchi Technique - A Review GuideA.BalaramNaik1, Dr.A.Chennakesava Reddy2, Dr.B.Balakrishna31Sr.Asst.Prof of Mech Engg, JNTUHCE Sulthanpur, Medak Dist2Professor of Mech Engg, JNTUHCE Hyderabad, Kukatpalli,3Assoc. Professor of Mech Engg, JNTUKCE Kakinada,Abstract:- Material characteristics and welding parameters play a very important role in determining the qualityof a weld bead. Duplex stainless steel (DSS) consists of approximately equal proportions of ferrite (δ) andaustenite (γ) phases. The DSS joint quality can be defined in terms of mechanical behavior, heat input, heat-cooling rate, weld oxide formation, sigma phase formation in weld metal and base metal. Different weldingprocess is used with the aim of obtained a best welding joint with the desired input parameters, good mechanicalproperties with minimum defects. Generally welding thermal cycle, dual torch, aging, heat treatment techniquesare more influence on quality of weld joint. In order to determine optimize process, design of experiment andcomputational network are widely using nowadays. A comprehensive review of the application of thesetechniques in the area of welding on different grades of duplex stainless steel has been introduced here in. Thispaper was classified according to the output features of the weld i.e. to optimize the mechanical properties bychanging the relative amount of ferrite, austenite and martensite content in base metal and weld metal. Thisreview shows many investigations and effects of phase transformation, heat treatment, dual torch technique onduplex stainless steel weldments and examined microstructure analysis at different experimental conditions inorder to obtain superior welded joints.Keywords: - Duplex stainless steel; Welding, Quality of weld metal; Ferrite-Austenite; Taguchi, Optimization.I. INTRODUCTIONDuplex stainless steel(DSS) typically comprises microstructure consisting approximately equalproportion of Body-centered cubic ferrite (δ) and face centered cubic austenite (γ),which offers greatermechanical strength and high corrosion, pitting and fatigue resistance than most types of stainless steel. Duplexstainless steel is a common structural material in the oil, gas, manufacturing industries and has specialapplication in chemical, wastewater, marine engineering field. An important limitation of the DSS is itsmaximum temperature of service, below 3000C,due to the problem of brittleness at 4750C.The performance ofDSS can be significantly affected by welding technique-induced phase transformation and understanding of theevolution of microstructure during welding is need in order to predict the final weld properties. The quality ofDSS weld joint is directly influenced by heat input parameters, type of welding process and type of technique,therefore welding can be considered as a multi-input multi-out put process. By changing chemical compositionof base metal and filler metal of duplex stainless steel, it requires time-consuming trial and error developmentmethod for choosing best weld parameter to produce a welded joint that closely meets the required specificationof joint. The various optimization methods of different welding process can be applied to define the desiredoutput variables on DSS through developing design of experiment (DoE) technique, taguchi technique andstatistical approaches have been used to such optimization. Sigma phase formation on duplex stainless steelweld metal is greatly influence by single pass and multi pass gas tungsten arc welding (GTA) without fillermaterial in argon gas. Activated tungsten inert gas(ATIG) welding technique, which control the ferrite/austenitecontents of the weld metal are very important for DSS to avoid degrade the strength and corrosion resistance.The optimal mechanical properties were obtained when precipitation of sigma and the γ-to-δ ferritetransformation are suppressed, i.e., at 10500C.Ni percentage on filler metal and weld oxide formation on DSSalso improve the quality of weld and develop corrosion fatigue resistance. Effect of solution heat-treatment onDSS weld metal will increases pitting resistance and content of γ-phase in weld bead and in heat affected zone(HAZ) increases which promotes weldability, excellent mechanical properties.In this paper a comprehensive detail review of the application of different optimize technique ispresented. This literature review shows the relations between the welding input parameters and the output weldbead variables, the paper also present the characteristic optimization of the different welding process on duplex
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 27stainless steel through experimental microstructure analysis. The classification of the literature review will beaccording to the weld joint features.II. PHASE FORMATION IN DSS WELD BEADThe performance of duplex stainless steel can be significantly affected by welding induced phasetransformations; hence formation of ferrite, austenite phases in weld metal and base metal after performingwelding process is very important. Controlling of weld-bead phase is essential as the mechanical properties ofwelds are affected by the weld-bead phase. Therefore, it is clear that precise selection of the process parametersis necessary.2.1 Ferrite formationW.Zhang and T Debray  have highlighted to developed ferrite formation in duplex stain less steel byone-dimensional numerical diffusion model. DSS are two phase alloys consisting of approximately equalproportions of ferrite (δ) and austenite (γ) phase with high toughness, good weldability, satisfactory resistanceand high tensile strength. Investigation on heat affected zone (HAZ) has been done to understand the phaseformation, phase fraction, grain size during the weld heating and cooling cycles.By using the numerical diffusion model and computed heating rates, time-temperature-transformation(TTT) and continuous-heating transformation (CHT) diagrams for DSS were constructed and the kinetics ofthe γ-δ transportation at various locations in the HAZ could be calculate and validate by comparing thecalculated result with data obtained using a spatially resolved X-ray diffraction (SRXRD) technique.2205 DSSconsists of alternate layers of 54% δ ferrite and 46 % γ-austenite phases has been solution annealed attemperature of 1338 K for a period of 2.5 hours following by water quenching to ambient temp to achievestarting microstructure. The initial nitrogen concentration and total nitrogen concentration can be known usinggoverning equations of nitrogen diffusion.𝜕𝑁𝜕𝑡= 𝐷𝛿𝜕2 𝑁𝜕𝑋 2in δ (0 <x< M)(1)𝜕𝑁𝜕𝑡= 𝐷𝛾𝜕2 𝑁𝜕𝑋 2in γ ( M<x<𝑥 𝛾 )Where N is the nitrogen concentration, t is time, 𝐷𝛿 𝑎𝑛𝑑 𝐷𝛾 are the diffusion coefficients of nitrogen in the δand γ phases respectively.2.2 Thermodynamics of γ-δ transformationThe equilibrium fraction of(γ)has been experimentally measured in the literature  by Hertzman forthe number of duplex stainless steels. The relationship of 𝑓𝛾 as a function of temperature and composition isgiven as𝑓𝛾=0.01[75-6.8× 10−15× 𝑇5+ 190 𝐶 𝐶 − 0.03 + 6 22 − 𝐶𝑟𝐶 + 9 𝑁𝑖 𝐶 − 5 + 6.5 3 − 𝑀𝑜 𝐶 +160(𝑁𝐶 − 0.15)] (2)Where𝐶 𝐶is the carbon concentration, 𝐶𝑟𝐶is the chromium concentration 𝑁𝑖 𝐶is the nitrogenconcentration. The concentration of C, Cr, Ni, Mo and N in Eq (2) are the average concentrations of elements inthe base metal determining by chemical analysis. It found that 1338 K is only a nominal start temperature andnot the equilibrium temperature for the start of the γ-δ transition.The spatially resolved X-ray diffraction (SRXRD) technique was used to obtain real-time kinetic data for the γ-δtransformation during welding gas tungsten arc (GTA) welds were made on 2205 duplex stainless steelcylindrical bar samples .During welding sample was irradiated with a high-intensity synchrotron beam, and thediffracted beam was collected to determine the crystal structure at discrete location. Additional details of theSRXRD experiments are available elsewhere [4, 5].It is found that the overall transformation rate is 30 % fasterwhen the starting structure is uniform. The transformation rate increase with temperature and the non-uniformstarting structure delays the completion of the phase transformation.2.3 Sigma phase formation on DSS.Yutaka S.Sato and Hiroyuki  have extended their study and examined the effect of chemical drivingforce on sigma phase formation in duplex stain less steel weld metals with different chemical compositions. Theeffort of crystallographic orientation relationship at δ/γ interface on sigma phase formation in a DSS weld metal,where the chemical element distribution is relatively uniform because of rapid cooling during weld thermalcycle. The chemical composition(Wt %) isFe-25.05%,Cr-4.7%,Ni-1.90%,Mo-0.4% of 50 × 150×90 mm in sizeof base metal plate was welded by sigle pass gas tungsten arc (GTA) welding without filler material in argongas. Relationship between the pair of deviation angle ∆𝜃 𝐾−𝑆 of intergranular-austenite and the misorientation atprior ferrite grain boundary in the weld metals and relationship between frequency of α/γ interfaces and the
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 28deviation angle ∆𝜃 𝐾−𝑆 are examined. Sigma phase forms preferentially at one side of ferrite/austenite interfacealong intergranular austenite in a DSS weld metal annealed at 1100K.The minimum deviation angle forsigma phase formation is strongly influenced by the interfacial energy and the coherency of ferrite/austeniteinterface. High coherent and low energy ferrite/austenite interface can delay sigma phase formation.2.3. Weld oxide formation on DSSE.M.Westin and O.A.Olsson  have continued their previous study and successfully investigated theeffect of weld oxide have a strong influence on corrosion resistance of Duplex stainless steel. Chromiumdominates in the weld oxide formed at high temperature and reaches a maximum above 9000C related thechromium reduction in heat tint formed at the highest temperatures to evaporation of chromium oxide, CrO-3.Best corrosion resistance accurse by mechanical cleaning followed by pickling.Higher alloyed grade steels does not affect the corrosion resistance as compare with lower alloyed grade steels.Gas tungsten arc welding (GTAW) was performed on different welded duplex stainless steel grades (LDX 2101,2304, 2205 and 2507) and followed by corrosion testing, ferroxyltest, electron probe micro analysis-ray photoelectron spectroscopy test were carried out to examined the effect on corrosion resistance and weld oxideformation.The influence of nitrogen, nickel, manganese on heat tint formation is more . After examined allexperimental test on all samples it shows that discoloration only for the welds in nitrogen-containingatmosphere, not those with argon. The reason seems to be the manganese or chromium oxynitrides formed in theformer case and appear to be responsible for the staining.III. HEAT TREATMENT ANALYSIS ON DSS.Welding is usually done with the aim of getting a welded joint with best mechanical properties.On any type of material, the property of base metal and quality of welded joint is greatly influence by the heattreatment process. The effect of heat treatment also have great change in microstructure and it balance theferrite, austenite content in the weld metal and in heat affected zone (HAZ) which promotes weldability andexcellent mechanical properties.2.4 Effects of solution heat-treatment on DSS welds.Soon-Tae Kim and Seok-Hwan Jang  have presented an experimental analysis of the effects ofsolution heat-treatment on hyper duplex stain less steel (HDSS) weldments. HDSS such has UNS 532707 isdefined as a highly alloyed DSS with a PREN Value is greater than 45.After performing a solution heat-treatment on hyper DSS weld metal with an Argon shielding gas supplemented with N2,the pitting resistance-phase in the weld metal and in heat affected zone was increase which promotes weldability, excellentmechanical properties. Post weld heat treatment (PWHT) is very important to control over the balance of a α, γphases in the weld metal (WM) and HAZ. Nitrogen (N) is a strong γ-stabilizer and it increase the temperature atwhich the transformation of α-to γ phase occurs.PREN = wt % Cr + 33 (wt % Mo + 0.5 × 𝑤𝑡 % W) + 30 × wt. %N. (3)The formula in Eq (3) for DSS has been used by several researchers to investigate DSS’s resistance tolocalized corrosion .Metallographic examination, polarization test, critical pitting temperature test, scanning electronmicroscope and energy dispersive spectroscope (SEM-EDS) analysis and transmission electron microscope(TEM) analysis of Cr2N precipitate were carried out and examined the effect of heat treatment on the resistanceto pitting corrosion of a HDSS welds. The phase diagram and equilibrium fraction of each phase were calculatedagainst the temperature for the HDSS alloy using a commercial thermo calculation software package. Basedupon the PRENγ and PRENα values calculated using a N factor of 30,pitting corrosion in the weld metalsand HAZ’S in the solution heat-treatment HDSS tube after welding was selectively initiated at the α-phase,irrespective of the chemical compositions of the shielding gas. The pitting corrosion was finally propagatedfrom the α-phase to the γ-phase.2.5 Effects of Aging on DSS weldments.Omyma Hassan Ibrahim and Ibrahim Soliman Ibrahim  have explain about the effect of aging heattreatment at (650,750 and 8500C) on2205 duplex stain less steel after performing TIG (Tungsten inert gas)welding technique. DSS weldments are the degradation of corrosion and mechanical properties within certainhigh temperature due to the micro structural changes. In comparison to austenite stainless steel, precipitation ofsigma phases in DSS accurse within the ferrite phase at shorter time, at higher temperature and with largervolume fractions.Material with dimension of 55 mm × 10𝑚𝑚 × 4.5𝑚𝑚 were subjected to solution heat treatment at10500C and 11500C respectively for 1 hour and then water quenched and then isothermal aging treatment was
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 29applied to base and weld metals at 6500,7500and 8500C for 3hour followed by furnace cooling. Microstructureanalysis, impact properties, load time plots for austenite stainless steel and duplex stainless steel weldmentswere verified and found that impact energy is higher for DSS in the un-aged conditions. The degree ofembrittlement is greater with the increases of the aging temperature.SEM examination reveals that thereduction in impact energy due to aging is associated with the formation of shallow ductile dimples andcleavage facets on the fracture surface of 316 L and duplex stainless steels, respectively.2.6 Welding thermal cycles on DSS.HuaTan and Zhiyuwang  have investigated the welding thermal cycle on 2305 DSS.Duplexstainless steel are widely used as alternatives to austenite stainless steels and nickel based alloys, which consistsof approximately equivalent amount of γ and α-ferrite with an excellent combination of mechanical strength andcorrosion. Different welding thermal cycles from single-pass to triple pass were performed on two kinds of 2304DSS. The most typical problems of welded DSS are associated with heat-affected zone (HAZ), not with weldmetal zone (WMZ), since the properties of WMZ could be modified by using high-alloyed filler metal and N2containing shield gas. More sophisticated and complicated microstructure evolution in HAZ during multi-passwelding.Material is divided into several blooms with a dimension of 150mm×100mm ×42mm is heated invacuum furnaces from 900 to 12000C temperature range and then reheated at 12500C for 2 hours and hot-rolledin to 12 mm thickness plates. Chemical composition of DSS.Chemical composition of two kinds of duplex stainless steel 2304 (Wt %)Element Cr Mo N N Cu C2304-A 23.06 0.31 0.13 4.03 0.29 0.0212304-B 23.82 0.91 0.18 4.50 0.35 0.02Element Mn Si P S Fe2304-A 1.56 0.40 0.010 0.004 Bal2304-B 1.52 0.38 0.008 0.004 BalThe above two grade specimens were solution –annealed for 12 mints at 12500C and 10500Crespectively quenched in water. Electrochemical measurements-critical pitting temperature test is done at leastthree times for the same specimen and microstructure analysis also carried and it so that all the welding thermalsimulated specimens exhibited impaired microstructure and pitting corrosion resistance compared with thecorresponding base metal. As welding pass increases CPT value increases the ferrite phase fraction decrease andimprovement of the microstructure and pitting corrosion resistance. PREN (pitting resistance equivalentnumber) increases.2304-B DSS with higher alloyed specimens  showed better microstructure and pittingcorrosion resistance than the corresponding 2304-A specimen.3.4. Hydrogen-enhanced cracking of DSS WeldsM.C.Young and S.L.I.Chan  have continued their investigation of the effects of hydrogen, nitrogenaddition during laser welding to improve the weldability of duplex stainless steel. The susceptibility decreasedwith increasing austenite content in the weld metal of DSS. Slow displacement rate tensile tests were carried outto investigate the effect of hydrogen embrittlement on notched tensile strength (NTS) and fracturecharacteristics of 2205 DSS weld. Plastic deformation occurs more easily in low alloy DSS, resulting growth ofstress corrosion cracks in the austenite. In highly alloyed DSS the strength of austenite is higher and cracking inthe ferrite in chloride solution is promoted. By controlling the heat input and interpass temperature duringwelding are required to correct the α/γ ratio in the DSS weld. Laser welding offers many advantages over theconventional arc welding process on DSS, by varying welding parameters γ phase content in the fusion zone ofa 2205 DSS is increases.Microstructure observations, charpy impact test, notched tensile test, fracture morphology were carriedout after laser welding on DSS and found the α/γ ratio in the fusion zone was drastically increased.Theeffect of N addition during laser welding also improved the weld’s ability to resist impact fracture. Hydrogenembrittlement susceptibility is more obvious for the specimens containing a greater amount of α phase.SEMfractographs shows that all specimens underwent a significant change in fracture mode from ductile in air tomainly quasi-cleavage fracture in H2.3.5. Influence of heat input on DSS welds.M.Yousefieh and M.Shamanian have presented an experimentally the effect of heat inputvariations on the microstructure of a duplex stainless steel UNS S32760 in artificial sea water media.Approximately 0.95 k J / mm of heat input have the best corrosion characteristics which are the result for the
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 30lack of deleterious phases such as sigma and Cr2N and balanced ferrite –austenite proportion. The pulsed currentof gas tungsten arc welding (GTAW) process has a numerous advantages over the conventional GTA process,the ferrite-austenite ratio in base metal as well as in weld metal depends on the energy input in welding. Afterperforming welding on four different size of DSS pipe, metallographic test done by scanning electronmicroscope (SEM) and energy dispersive X-ray spectrometer (EDX) test were performed to reveal the chemicalcomposition of the phases present in the microstructure and polarization curves of various specimens can beanalyzed.The results of various test shows that formation of sigma and Cr2N phases reduced corrosion potential.The lower austenite content due to the high heat input and sufficient time for ferrite-austenite transformation.IV. MECHANICAL PROPERTIES.Welding is usually done with the aim of getting a welded joint with excellent mechanical properties.By changing welding technique, input parameters, heat treatments, chemical composition of duplex stainlesssteel, the welded joint may be examined and investigate to improve their mechanical properties. To determinethese welding combinations that would lead to excellent mechanical properties for DSS weldments. Differenttechnique, methods, approaches and composition have been used to achieve this aim. The following is a reviewof some articles that utilized these techniques for the purpose of optimizing the welding process for DSS inorder to achieve the desired mechanical properties of the welded joint.4.1. Mechanical behavior in annealed DSS welds.RiadBadji and MabroukBouabdallah  have examined the effect of annealing treatment of 2205DSS on mechanical properties. The tube type DSS material of 170 diameter and 7 mm in wall thickness iswelded using a gas tungsten arc welding process in multi pass with Ar+2%N2 shielding gas and ER 2209 fillermetal. After welding, series of heat treatment were performed from 80000C to12000C and then etched withsolution like 10 ml HNo3, 20ml glycerol and 30 ml Hcl.By ZEISS optical microscope, optical micrograph of welded specimen over heated parts of the HAZ, andpartially annealed region of the HAZ at different ranges was done. The EDX analysis technique has been used toidentify the phases constituting each microstructure region . The best combination of strength stress σ =775MPa and elongation δl=36.45 % is obtained after annealing at 10500C.Asignificant change in the toughness andtensile properties has been observed as a consequence of precipitation phenomena or an increase of ferritecontent. The optimal mechanical properties were obtained when precipitation of sigma and the γ-to-δ ferritetransformation are suppressed i.e. at 10500C.4.2. Activated TIG welding on DSS.Tsann-ShyiChern and Kuang-HungTseng  have continued their study and examined the tensilestrength. The effect of the specific fluxes used in the Activated tungsten inert gas welding process on 6 mmthick duplex stainless steel also investigated. Penetration during TIG welding process depends upon weldcurrent, weld speed, thickness of metal, material, flux used and type of electrode. By using activated flux, the200%-300% deep penetration takes place. The technique that control the ferrite /austenite contents of the weldmetal are very important for DSS to avoid degrade the strength and corrosion resistances. Effect of activatedTIG welding on (surface, weld morphology, angular distortion, ferrite and austenite content) with flux andwithout flux has be experimental examine was done and finally mechanical properties found are tensile strengthσ =765 Mpa, and 35 % elongation. By using SiO2,MoO2 and Cr2O3 flux penetration capacity increased andimproved mechanical strength. The greater weld depth-to-width ratio take place with activated TIG weldingprocess as compare with the normal TIG welding . As a result arc voltage increases and the ferrite content inthe welded bead is decreases.4.3. Corrosion fatigue of DSS welds.S.A Tavara and M.D.Chapetti  have stated that the duplex stainless steel of two phasemicrostructure austenite and delta ferrite in approximately similar percentages have greater yield strength thanaustenitic stainless steels. Welded parts has less resistance than base metal by control of carbon content(lowcarbon) and welding conditions to ensure austenite formation can make corrosion resistance of DSS equivalentto base metal.Austenite/ferrite contents of welded DSS is dependent upon electrode composition, Ni plays animportant role in the balance as austenite promoter. Corrosion fatigue in welded joints is considered a verydangerous type of propagation of defects in materials that are subjected to dynamic loads. Welding hasperformed on four different composition of base metal with four different filler metal (electrode A,B,C,D) andtested mechanical properties after heat treatment was made to 10500C for 1 hour. Three point bending fatiguetest were carried out in a load control walking –beam fatigue machine in air and sea water of different frequency
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 31and found that Ni content has a direct relation to the number of cycles necessary to reach a depth of 1.5mm.The environmental contribution to the crack growth rate is:(da/dN)cf= (da/dN)e – (da/dN)rWhere (da/dN)e is the measured crack growth rate and (da/dN)r is the reference crack growth rate,corresponding to pure mechanical fatigue in air.V. OPTIMIZATION TECHNIQUES.Different methods, approach and techniques have been used to achieve excellent weld bead with besttensile strength on DSS, Low carbon steel, high carbon steel. The follow is a review of some researches thatutilized these techniques for the purpose of optimizing the welding process.2.7 Taguchi technique.Juang and Tarng have adopted a modified Taguchi method to analyze the effect of each weldingprocess parameter (arc gap, flow rate, welding current and speed)on the weld pool geometry (front and backheight, frontand back width) and then to determine the TIG welding process parameters combination associatedwith the optimal weld pool geometry. It was experimentally reported that, the four smaller-the-better qualitycharacteristics,’ four responses’ of the weld pool in the TIG welding ofS304 stainless steel of 1.5 mm inthickness are greatly improved by using this approach.Lee HK and Han HS.  have used the Taguchi method and regression analysis in order to optimizeNd-YAG laser welding parameters (nozzle type, rotating speed, title angle, focal position, pumping voltage,pulse frequency and pulse width) to seal an iodine-125 radioisotope seed into a titanium capsule. The accuratecontrol of the melted length of the tube end was the most important to obtain a sound sealed state. It wasdemonstrated that the laser pulse width and focal position were the laser welding parameters that had thegreatest effects on the S/N ratios of the melted length. The optimal welding conditions were obtained at a pulsewidth of 0.86 ms and a focal position of 3.18–3.35 mm. Furthermore, confirmation experiments were conductedat the optimal welding conditions, it can be said that the titanium tube ends were sealed perfectlyLaser butt-welding of a thin plate of magnesium alloy using the Taguchi method has been optimized byPanet al. . They studied the effect of Nd-YAG laser welding parameters (shielding gas type, laser energy,conveying speed, laser focus, pulse frequency and pulse shape) on the ultimate tensile stress. Their resultindicated that the pulse shape and energy of the laser contributed most to thin plate butt-welding. It was foundthat the optimal combination of welding parameters for laser welding were argon as a shielding gas, a 360 Wlaser energy, a work piece speed of 25 mm/s, a focus distance of 0 mm, a pulse frequency of 160 Hz and type IIIpulse shape. It was also found that the superior ultimate tension stress was169 MPa at an overlap of the weldingzone of approximately75%.2.8 Response surface methodology (RSM).Wang and Rasmussen  have investigated the inertia welding process of low-carbon steels usingRSM, with the purpose of establishing an empirical functional relationship between the process parameters (theaxial pressure, the initial rubbing velocity and the total moment of inertia) and the breaking strength of the joint.It was concluded that a relatively wide range of operating conditions would produce successful welds. Also,they observed that the average micro hardness at the weld was about 27% higher than the base material and theideal weld should be made with the least possible amount of kinetic energy as long as full penetration at theinterface is achieved.Benyounis and Bettamer have proposed models using RSM to investigate the effect of weldingparameters in SAW(welding current, arc voltage and welding speed) on the impact strength at two testingtemperatures of 50 _C and27 _C. The aim was to predict and optimize the impact strength of the spiral-weldedjoints with respect to the process parameters. It was observed that the welding current was the most significantfactor associated with the impact strength, then the welding speed, whereas the welding voltage has nosignificant effect within the factors domain investigated. They listed the optimal welding conditions that wouldlead to acceptable impact strength with improving the process productivity2.9 Artificial neural networks (ANN).Control of distortion and overall quality of welds were investigated by Casalino et al.  in order toselect the GMAW process parameters that minimize thermal deformation and evaluate weld quality. Theyintegrated the artificial intelligence techniques and FEM with the aid of experimental trials of bead-on-platewelds. The base metal was 1.6 mm thick low-carbon steel, a 0.9 mm diameter copper-coated wire was used asan electrode with a shielding gas consisting of a 75% Ar–25% CO2 mixture with flow rate of 10–15 ft3/h.ANN was used at first to link the process parameters to the geometry of the molten zone, which allowed thegeometries throughout a range of process parameters to be calculated. Then FEM was applied to predict the
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 32residual stress value and distortion in the welded joint. Finally, fuzzy C-means clustering algorithm was appliedto evaluate the quality joints. Mathematical models for GMAW were constructed. Experimentally butt weldedjoint were validated. It was concluded that the experimental result are in good agreement with the mathematicalmodel.5.4. Dual torch technique on DSS welds.Z.Sun and M.Kuo  have investigated the effect of the dual-torque technique on the microstructurechanges and corrosion properties of duplex stainless steel were examined. Ferrite percentage is very importantto reduce stress-corrosion cracking resistance, therefore to control this technique uses two welding torches’ (aplasma welding torch followed by a gas tungsten arc (GTA welding torch) simultaneously during welding.SAF2205 DSS with 5.5 mm thickness material were performed dual torch technique, potentiodynamic measurementsand electro chemical impedance spectroscopy were performed. Polarization curves of the base metal and weldmetal are examined at different torch pitch ( 25,30 and 35 mm).Corrosion rates for the DSS welds alsoexamined and demonstrated the potential of using dual torch plasma welds to improve weldability of duplexstain less steels.VI. COMPARISON BETWEEN THE OPTIMIZATION TECHNIQUESDerived from the above literature review some insight has been gained into the use of DoE, ANN, Dualtorch technique, Taguchi method and other techniques for modelling and optimizing different welding processeson DSS. It was noted that Taguchi performs better than other techniques, especially ANN and RSM, when alarge number of experiments are not affordable. The trend in the modelling using Taguchi method has a loworder non-linear behavior with a regular experimental domain and relatively small factors region, due to itslimitation in building a model to fit the data over an irregular experimental region. This ability is powerful inidentifying the insignificant factors main effect, insignificant interactions or insignificant quadratic terms in themodel and thereby can reduce the complexity of the problem. On the other hand, this technique required gooddefinition of ranges for each factor to ensure that the response(s) under consideration is changing in a regularmanner within this range.The Taguchi method is one of the powerful optimization techniques comparing with RSM, ANN andDual torch technique which characterize with improving the product quality and reliability at low cost.However, RMS analysis approach of SN may lead to non-optimal solutions, less flexibility and the conductionof needless experiments.2.10 Comparison between RSM and ANNs Techniques.Table 1Comparison TechniqueANNs RSMTime taken long MediumExperimentaldomainirregular IrregularUnderstanding Difficult ModerateOptimization Through model StraightAvailability insoftwareAvailable AvailableApplication Rarely Rarely2.11 Comparison between Taguchi and Dual torch Techniques.Table 2Comparison TechniqueTaguchi Dual torchTime taken Short LongExperimentaldomainRegular RegularUnderstanding Normal EasyOptimization Through model StraightAvailability insoftwareAvailable AvailableApplication Frequently Not frequently
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 33Table 1 and Table 2presents a comparison between the above mentioned common modelling /optimizingmethods based on this literature review.VII. CONCLUSION1) In this paper the characteristics of duplex stainless steel and their mechanical behaviors, phasetransformation from ferrite to austenite and their limitation, advantages in base metal as well as in weldmetal was examined. Different welding process on DSS was proposed and it found that the overall phasetransformation rate is fastest when the starting structure is uniform and non uniform starting structuredelays the completion of the transformation.2. An explanation for the difference in heat treatment process and their effort on DSS weldments wasproposed based on (TEM) analysis, (SEM-EDS) analysis. The effort of nitrogen, aging, hydrogen-enhancing on DSS weld were examined and investigate the pitting resistance equivalent number(PREN).By performing heat treatment process-phase in the weld metal and in the HAZ is increases whichpromotes weldability.3. This study systematically investigate the effects of different fluxes on surface appearance, weldmorphology, ferrite/austenite content and mechanical properties of duplex stainless steel after performingdifferent experimental methods with varying chemical composition for base metal and feller metal. It wasfound that the optimal mechanical properties were obtained when precipitation of sigma and the γ-to-δferrite transformation are suppressed i.e. at 10500C and 8.9% Ni electrode showed better performance.4. The optimization method covered in this literature survey is appropriate for selecting design ofexperiment, control and optimizing the different welding process. The survey reveals that the adoption ofRSM, ANNs, Taguchi and a Dual-torch technique on DSS was proposed. Generally there is a lack ofcomparative study regarding the performance of the optimization method. It was found that the Taguchimethod is one of the powerful technique which characterize with improving the product quality andreliability at low cost. Combining two optimization techniques, such as RSM and Taguchi on Duplexstainless steel (DSS) would reveal good results for finding out the optimal welding conditions .Futurework should focus on the application of these optimization techniques to find best optimal weldingprocess for DSS, at which the process could be consider safe and economical.REFERENCES. W.Zhang,T.DebROY,T.A.Palmer,Modeling of ferrite formation in a duplex stainless steelweldconsidering non-uniform starting microstructure,Elsevier,2005.. Mundra K,DebRoy T,Kelkar K.M.Numer.Heat Transfer A,1996;29:115.. Hertzman S,Roberts W,Lindenmo M.In: Proceedings of duplex stainless steels 86, The Hague,TheNetherlands;1986.p.257.. Palmer TA,Elmer JW,Wong J .Sci.Tecnol. Weld .Joining 2002;7:159.. Palmer TA,Elmer JW,Babu SS.Mater.Scieng.A 2004;374:307.. Yutaka S.Sato and Hiroyuki Kokawa,Preferential precipitation site of sigma phase in duplex stainlessstell weld metal, Pergamon, 1998.. Y.S.Sato,H.Kokawa,andT.Kuwana,Sci.Technol.Weld.Join.in press (1998).. E.M.Westin,C.-O.A.Olsson,S.Hertzman,Weld oxide formation on lean duplex stainlesssteel,Elsevier,(2008).. S.Hertzman,R.Petterson,L.Liu,S.Hanstrom,B.Brolund,Controlled nitrogen uptake during hightemperature annealingofstainlesssteels,in:M.Speidel,C.Kowanda,M.Diener(Eds),Proceedings ofinternational Conference on HNS 2003,High Nitrogen Steels,vdf Hochschulverlag AG an der ETHZurich,2003,pp.217-228.. Soon-Tae Kim,Seok-Hwan Jang,In-Sung Lee,Yong-Soo Park,Effects of solution heat-treatment andnitrogen in shelding gas on the resistance of pitting corrosion of hyper duplex stainless steelwelds,Elsevier,(2011).. M.Barteri,M.G.Mecozzi,I.Nembrini,DuplexStainlessSte es94,Vol.3,Glasgow,Scotland,1991.paper 60.. U.Heubner,M.Rockel, Werkst.Korros.37(1986) 7-12.. Omyma Hassan Ibrahim,Ibrahim Soliman Ibhahim,Effect of aging on the toughness of austentic andduplex stainless steel weldments,Elsevier,2011.. George E.Totten:Steel Heat Treatment,Metallurgy and Technologies,John Wily and Sons Inc.,NewYork,2007.. Hua Tan,Zhiyu Wang,Yiming Jiang,Jin Li,Influence of welding thermal cycles on microstructure andpitting corrosion resistance of 2304 duplex stainless steels,Elsevier,2012.. H.Tan,Y.M.Jiang,B.Deng,Effect of annealing temperature on the pitting corrosion resistance of superduplex stainless steel UNS S32750,Mater.Charater.60(2009)1049-1054.
Characteristics Optimization of Different Welding Processes on Duplex…www.ijeijournal.com P a g e | 34. M.C.Young,S.L.I.Chan,Hydrogen-enhanced cracking of 2205 duplex stainless steelwelds,Elsevier,2004.. M.C.Young,S.L.I.Chan,L.W.Tsay,Fatigue Crack Growth Behaviour of 2205 Duplex Stainless Steel inCorrosive Environments,Mater.Sci.Eng.,A,submitted for publication.. M Yousefieh,M Shamanian,Influnce of heat input in pulsed current GTAW process on microstructureand corrosion resistance of duplex stainless steel welds,ScienceDirect 2011.. Riad Badji,Mabuouk Bouabdallah,Phase transformation and mechanical behavior in annealed 2205duplex stainless steel welds,Elsevier,2008.. Zucato I,Moreira MC,Machado IF,Lebrao SMG.Microstructural characterization and the effect ofphase transformations on toughness of the UNS 31803 duplex stainless steel aged treated at 8500C.Mater Res 2002;5(3):385-9.. Tsann-Shyi Chern,Kuang-Hung Tseng,Hsien-Lung Tsai,Study of the characteristics of duplex stainlesssteel activated tungsten inert gas welds,Elsevier,2011.. Huang HY,Shyu SW,Tseng KH,Chou CP.Elevation of TIG fluxwelding on the characteristics ofstainless steel.Sci Tecnol Weld Join 2005;10(5):566-73.. S.A.Tavara,M.D.Chapetti,J.L.Otegui,C.Manfredi,Influence of nickel on the susceptibility to corrosionfatigue of duplex stainless steel welds,Elsevier,2001.. Krausz K.The Development of the Constitutive Law of Crack Growth in CorrosionFatigue.In:Hadbook of Fatigue Crack Propagation in Mettalic Strucyures,3.1.3,1994.. Juang SC,Tarng YS.Process parameters selection for optimizing the weld pool geometry in thetungsten inert gas welding of stainless steel.J Mater Process Tecnol 2002;122:33-7.. Lee HK,Han HS,Son KJ,Hong SB.Optimization of Nd-YAG laser welding parameters for sealing smalltitanium tube ends.J Mater Sci Eng 2006;A415:149-55.. Pan LK,Wang CC,Hsiso YC,Ho KC.Optimization of Nd-YAG laser welding onto magnesium alloy viaTaguchi analysis.J Opt Lacer Technol 2004;37:33-42.. Wang KK,Rasmussen G.Optimization of inertia welding process by response surface methodology.JEng Ind 1972;94(4):999-1006.. Benyounis KY,Bettamer AH,Olabi AG,Hashmi MSJ.Prediction the impact strength of spiral-weldedpipe joints in submerged arc welding of low carbon steel.In: Proceedings of IMC21,1-3 September2004.Limerick;2004.p.200-10.. Casalino G,Hu SJ,Hou W.Deformation prediction and quality evaluation of the gas metal arc weldingbutt weld.J Eng Manuf 2003;217(part B):1615-22.. Z.Sun.M.Kuo, I.Annergren,D.Pan,Effect of dual torch technique on duplex stainless steelwelds,Elsevier,2003.